High carbon high chromium Steel D 2
D2 steel is an air hardening, high-carbon, high-chromium tool steel. It has high wear and abrasion resistant properties. It is heat treatable and will offer a hardness in the range 55-62 HRC, and is machinable in the annealed condition. D2 steel shows little distortion on correct hardening. D2 steel’s high chromium content gives it mild corrosion resisting properties in the hardened condition.
D2 Tool Steel
Cold-work tool steels include the high-carbon, high-chromium steels or group D steels. These steels are designated as group D steels and consist of D2, D3, D4, D5, and D7 steels. These steels contain 1.5 to 2.35% of carbon and 12% of chromium. Except type D3 steel, all the other group D steels include 1% Mo and are air hardened. Type D3 steel is oil-quenched; though small sections can be gas quenched after austenitization using vacuum. As a result, tools made with type D3 steel tends to be brittle during hardening. Type D2 steel is the most commonly used steel among the group D steels.
|Thermal expansion||10.4 x 10-6/ºC||20-100||-|
|Density||7.7 x 1000 kg/m3||0.278 lb/in3|
- DIN 1.2379
- NI KU
- B.S. BD 2
- ASTM A681
- FED QQ-T-570
- SAE J437
- SAE J438
- UNS T30402
D2 steels should be preheated very slowly to 815ºC (1500ºF) and then temperature can be increased to 1010ºC (1850ºF). They are then held at 1010ºC (1850ºF) for 20 to 45 minutes and air cooled (air quenched).
Forging of D2 steels can be done from 1065ºC (1950ºF) down to 954ºC (1750ºF). Do not forge below 926ºC (1700ºF).
D2 is supplied in the annealed and machineable condition. Re-annealing will only be necessary if the steel has been forged or hardened by the toolmaker. To anneal, heat slowly and uniformly to 900°C. Soak for three to four hours and allow to cool in the furnace to room temperature. Re-heat to 800-1040°C and again soak for three to four hours. Allow to cool in the furnace to room temperature.
It is preferable to heat the tools in a controlled atmosphere. If this is not possible, pack hardening is recommended. A reducing atmosphere is desirable. Pre heat the D2 tool steel component to 750-800°C. and allow to soak at this temperature. The tools may then be brought up to 1000-1040°C for air cooling, or 980°C for oil quenching. Soak thoroughly at the temperature for thirty minutes per 25mm of ruling section, then cool or quench accordingly. It is important not to exceed 1020°C when heating for hardening.
A popular grade for toolmakers, D2 is used in a wide variety of tool making applications. Typical applications include blanking dies and punches for sheet in stainless steel, brass, copper, zinc and hard abrasive materials generally. Other application include deep drawing dies, cupping dies, forming dies, sheet metal forming rolls, shear blades for strip and sheet including flying shears, circular cutters for cold rolled strip, trimmer dies, thread rolling dies, cold extrusion dies, broaches, plug gauges, ring gauges, special taps, straybolt taps, brick and tile mould liners, master hobs for cold hobbing plastic moulds and cut moulds for plastics.